The body is Plainsman L215. We used the 04DSDH firing schedule. The glaze is inexpensive to make so we have a 2 gallon bucket. It has good dipping much like a stoneware glaze so it is easy to apply quickly and evenly. For most terra cottas, body strength increases dramatically by cone 03. However the most transparent and glassy glaze surface happens at cone 06. Terra cotta bodies need to be bisque fired fairly low (e.g. cone 06) to have enough porosity to work well with dipping glazes. After cone 06 they generate increasing amounts of gases (as various particle species decompose within), for this reason the glazes can have more micro-bubble clouding or tiny dimples in the surface. This glaze has 2% iron oxide added as a fining agent to remove the bubbles. That iron also reddens the color and variegates the surface somewhat. Even though the surface character at cone 03 is not a smooth, it has a natural charm, and the color is very rich. And that piece has stoneware durability and strength.
Terra cotta bodies are typically fired between cone 06 and 04. That being said, many, like this Plainsman L215, develop richer color at cone 03 and fire much stronger. Glazes, of course, melt better and micro-bubbles pass through easier at cone 03. But this happens only if the body has not begun to decompose (and therefore generate a lot more gases of decomposition). Notice that crazing is beginning on the one of the left. Apparently the improved body:glaze interface and the development of better vitrification reduces the problem. Cone 03 is somewhat of a sweet-spot for this specific body, however firing higher begins decomposition processes that generate gases that disrupt the surface. Needless to say, accurate firing is needed to fire at cone 03 for ongoing success (because cone 02 is too high for this body, glaze will blister). Do you know what terra cotta actually is, if not click the link to learn more (this is a big topic).
G1916Q - Low Fire Highly-Expansion-Adjustable Transparent
An expansion-adjustable cone 04-02 transparent glaze made using three common Ferro frits (low and high expansion), it produces an easy-to-use slurry.
The term Terra Cotta can refer to a process or a kind of clay. Terra cotta clays are high in iron and available almost everywhere. While they vitrify at low temperatures, they are typically fired much lower than that and covered with colorful glazes.